Atomic displacement parameters for spessartine Mn~3~Al~2~Si~3~O~12~ and their lattice-dynamical interpretation
Gramaccioli, Carlo Maria; Pilati, Tullio; Demartin, Francesco; Acta Crystallographica Section B 58 (2002) 965–969; doi:10.1107/S0108768102017925

data_2103468
_publ_section_title
;
 Atomic displacement parameters for spessartine Mn~3~Al~2~Si~3~O~12~
 and their lattice-dynamical interpretation
;
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              965
_journal_page_last               969
_journal_paper_doi               10.1107/S0108768102017925
_journal_volume                  58
_journal_year                    2002
_chemical_formula_sum            'Al2 Mn3 O12 Si3'
_chemical_formula_weight         495.03
_chemical_name_systematic
;
 ?
;
_space_group_IT_number           230
_symmetry_cell_setting           cubic
_symmetry_space_group_name_Hall  '-I 4bd 2c 3'
_symmetry_space_group_name_H-M   'I a -3 d'
_audit_creation_method           'from SDP for Windows version 1.4  '
_cell_angle_alpha                90.0000000
_cell_angle_beta                 90.0000000
_cell_angle_gamma                90.0000000
_cell_formula_units_Z            8
_cell_length_a                   11.6300(10)
_cell_length_b                   11.6300(10)
_cell_length_c                   11.6300(10)
_cell_measurement_reflns_used    25
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      22.09
_cell_measurement_theta_min      12.20
_cell_volume                     1573.0(2)
_computing_cell_refinement       'CAD4 (Enraf Nonius)'
_computing_data_collection       'CAD4 (Enraf Nonius)'
_computing_data_reduction        'SDP for Windows'
_computing_molecular_graphics    'SDP for Windows'
_computing_publication_material  'SDP for Windows'
_computing_structure_refinement
'Full-matrix least-squares  (SDP for Windows)'
_diffrn_ambient_temperature      273
_diffrn_measurement_device       'CAD4 (Enraf Nonius)'
_diffrn_measurement_method       \w/2\q
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       0
_diffrn_reflns_limit_k_max       20
_diffrn_reflns_limit_k_min       0
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       0
_diffrn_reflns_number            2701
_diffrn_reflns_theta_max         40.00
_diffrn_reflns_theta_min         3.00
_diffrn_standards_interval_time  120
_diffrn_standards_number         1
_exptl_absorpt_coefficient_mu    5.31
_exptl_absorpt_correction_T_max  1.000
_exptl_absorpt_correction_T_min  0.703
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            orange
_exptl_crystal_density_diffrn    4.180
_exptl_crystal_description       '  [ENTER  SHAPE]'
_exptl_crystal_F_000             1912
_exptl_crystal_size_max          0.13
_exptl_crystal_size_mid          0.10
_exptl_crystal_size_min          0.10
_refine_diff_density_max         0.484
_refine_diff_density_min         0.000
_refine_ls_extinction_coef       0.0000
_refine_ls_extinction_method     'secondary Zachariasen'
_refine_ls_goodness_of_fit_all   0.652
_refine_ls_goodness_of_fit_obs   0.840
_refine_ls_matrix_type           full
_refine_ls_number_constraints    20
_refine_ls_number_parameters     40
_refine_ls_number_reflns         259
_refine_ls_number_restraints     0
_refine_ls_R_factor_all          0.036
_refine_ls_R_factor_obs          0.013
_refine_ls_shift/esd_max         0.034
_refine_ls_shift/esd_mean        0.008
_refine_ls_structure_factor_coef F
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_obs         0.016
_reflns_number_observed          289
_reflns_number_total             417
_reflns_observed_criterion       'F~o~ > 2.0 * 3.00 * sigma(F~o~)'
_cod_data_source_file            av0058.cif
_cod_data_source_block           I
_cod_original_sg_symbol_Hall     '-I 4bd 2ab 3'
_cod_database_code               2103468
_cod_database_fobs_code          2103468